CHAPTER 2. AREA SELECTIVE ATOMIC LAYER DEPOSITION
2.1 ATOMIC LAYER DEPOSITION
17 two consecutive dosing steps, to let unwanted molecules evacuate the chamber). The set of doses and purges represents an ALD cycle. By changing the number of cycles, it is possible to vary the thickness of the deposited film. ALD processes are often described in terms of their growth per cycle. Theoretically the growth per cycle (GPC) should be one monolayer per cycle but, in the practice, it can vary between 0.1 Å/cycle and 2 Å/cycle depending on process parameters, precursors reactivity, surface size and so on .
2.1.2 Binary ALD
The most part of atomic layer depositions requires the exposure of the substrate to only two precursors, let’s say A and B, often indicated as “reactant” and “co-reactant”: the sequence
“pulse A – purge – pulse B – purge” represents the cycle of the binary ALD, which is schematically portrayed in figure 2.1.
Figure 2.1: typical ALD process. (a) The substrate to be coated is placed in the reactor. (b) Precursor A is pulsed, and it reacts with the surface; (c) excess A precursor and reaction by-products are purged away. (d) Precursor B
is pulsed, and it reacts with the surface; (e) excess B precursor and reaction by-products are purged away.
(f) The cycle is repeated until the desired thickness is achieved .
2.1.3 ALD pros and cons
The advantages of ALD are several and the most important ones are listed below .
18 - It allows a precise thickness control at the Ångstrom level, due to the opportunity to
select the number of cycles.
- Films deposited by ALD tend to be very continuous, smooth and pinhole-free, since reactions develop completely during each cycle and no sites of the surface remain unfilled during film growth.
- The self-limiting nature of the reactions produce an excellent coverage of the substrate, leading to films which result extremely conformal to the geometry of the underlying structures, even for complex and high aspect-ratio substrates. In other words, it is not a line-of-sight process (such as PVD), in fact even if some surface areas react before than others (for example because of inhomogeneous precursor fluxes), the global reaction between precursor and substrate won’t stop until it has reached completion even in the areas less exposed.
Miniaturization process in the semiconductor industry has led to the necessity of continuous, defect-free films that must be deposited with high conformality and controlled thickness. No other techniques could satisfy these requirements as good as ALD.
The biggest weakness of ALD is the slow deposition rate, which derives from the long times involved in pulsing and purging, as well as the layer-by-layer nature of the deposition itself.
Most ALD rates fall within a range of 100÷300 nm/h . However, these rates strongly depend on the reactors design and the substrates (big and/or high aspect ratio substrates clearly need more time to be coated). CVD and PVD are certainly faster techniques, but they suffer from non-uniformity and non-conformality, respectively due to rapid surface reactions and shadowing effects.
2.1.4 Process parameters
The most important parameter in the ALD technique is the deposition temperature. ALD processes are carried at modest temperatures (normally below 350°C), more specifically in a well-defined range, which is denominated ALD temperature window and varies according to the precursors and the substrate involved .
Staying inside the window assures a self-controlled and saturated growth, whereas exceeding the limits of the window leads to no layer formation because of different effects, as shown in figure 2.2.
Figure 2.2: plot of ALD growth rate versus temperature. Temperature window is defined by T1 and T2.
- If the temperature is too low, either the thermal energy is not enough to overcome the activation energy of the reaction (low reactivity), or the precursor condensates on the surface through a non-ALD type deposition (condensation).
- If the temperature is too high, either the precursor thermally decomposes (decomposition), or it rapidly desorbs from the surface (after having been chemisorbed) because of too much thermal energy (desorption).
Other parameters to be considered for an atomic layer deposition are pulse and purge times, which indicate, respectively, the quantity of reactant and inert gas that enters the reactor chamber per cycle .
Short pulse time implicates incomplete reaction between precursor and surface sites of the substrate, which results in poor quality and uniformity of the film. On the other hand, long pulse time produces waste of precursor and can make some reactant particles stick to the top layer, event that compromises the reaction of the successive cycle. Besides, short purge time is not enough to clean up completely the by-products, whereas long purge time may provoke the entry of impurities.
2.1.5 Growth mechanism
Concerning the kinetic of the process, different growth mechanisms have been identified, in relation to what happens to the growth per cycle (GPC). The only differences in the trend of the GPC are registered in the very beginning of the growth, when the substrate is not fully
20 covered yet: with the increasing extent of deposition, in fact, the original substrate gives way to the first layer of the film to be deposited and the growth per cycle is expected to become constant in any case. As it can be observed in figure 2.3, the GPC can be classified as constant [2.3(a)], substrate enhanced [2.3(b)] or substrate inhibited [2.3(c)] .
Figure 2.3: proposed classification of ALD processes based on the initial growth per cycle.
(a) Constant GPC; (b) substrate enhanced GPC; (c) substrate inhibited GPC .
When the GPC is constant, the ALD is said steady. It is important to notice that in a steady ALD the physical quantity that stays constant is the amount of material deposited versus the number of ALD cycles, while in a steady CVD it is the amount of material deposited versus time (i.e. the growth rate) to be constant. In the substrate enhanced ALD, the GPC is higher in the beginning with respect to the steady state, while in the substrate inhibited ALD, the GPC is lower, but it gradually increases until it reaches the steady state.
At the origin of the third growth mechanism (GPC substrate inhibited) a model of islands growth has been proposed. According to this model, the substrate is not really reactive towards the ALD precursors, except for some active defective-areas: nucleation starts at these defective points and create “islands” which continue to grow regularly, i.e. laterally and symmetrically from the center .
2.1.6 ALD precursors
As it can be clearly noticed consulting scientific journals, there is a wide variety of materials that can be grown through atomic layer deposition, among which metals, semiconductors and insulators, in both crystalline and amorphous phases. Table 2.1 summarizes elements and various compounds (binary oxides, nitrides, sulfides) that can be obtained by the technique . Basically, the main limitation to the realization of a material via ALD is the availability of reactants that can interact with the surface through the appropriate chemical
21 pathway, in order to obtain that material. Precursors should be easily available or synthesized and not very expensive; furthermore, they should be volatile enough to be in the gas phase either at room temperature or upon moderate heating and, once in the gaseous state, they should not decompose until they have reached the surface of interest.
Finally, they must react with surface groups rapidly and they should interact aggressively with each other to reach the saturation stage in a short time and ensure a reasonable deposition time [20, 24].
Table 2.1: list of materials grown by ALD .
Oxides (ExOy) Nitrides (ExNy) Sulfides (ExSy)
C, Al, Si, Ti, Fe, Co, Ni, Cu, Zn, Ga, Ge, Mo, Ru, Rh, Pd, Ag, Ta, W, Os, Ir, Pt
Li, Be, B, Mg, Al, Si, P, Ca, Sc, Ti, V, Cr, Mn, Fe, Co, Ni, Cu, Zn, Ga, Ge, Sr, Y, Zr, Nb, Ru, Rh, Pd, In, Sn, Sb, Ba, La, Ce, Pr, Nd, Sm, Eu, Gd, Tb, Dy, Ho, Er, Tm, Yb, Lu, Hf, W, Ir, Pt, Pb, Bi
B, Al, Si, Ti, Cu, Ga, Zr, Nb, Mo, In, Hf, T, W
Ca, Ti, Mn, Cu, Zn, Sr, Y, Cd, In, Sn, Sb, Ba, La, W
All sorts of reactants in accordance with the aforementioned requirements have been tried in atomic layer depositions. The non-metal precursors are usually hydrides (H2O, H2S, NH3, AsH3). H2O and H2S show reactivity at reasonable temperatures (T < 500°C) and formation of suitable surface species to anchor the metal precursor, while NH3 and AsH3 have more limited reactivity. Among the metal precursors it is possible to remember metal halides (especially chlorides, widely applied for oxide, nitride and sulfide films formation), metal alkyls (which in some cases behave almost ideally in the formation of oxide and sulfide films), metal alkoxides, electropositive metals compounds and metal alkyl amides (as precursors for nitride films) .
To give a more practical example of reactants (and reactions) involved in a typical atomic layer deposition, it is possible to analyze one of the first substances grown by this technique,
22 namely aluminium oxide (Al2O3), which also is one of the most used materials in electronics applications .
Many reactions pathways exist, but two reactants are needed in any case, the first containing aluminum and the second containing oxygen. The most studied aluminum source is trimethylaluminum (Me3Al), which has been employed by different research groups using various oxygen sources, such as water (H2O), hydrogen peroxide (H2O2), nitrogen dioxide (NO2) and ozone (O3) [25, 26]. The reaction with water is:
2Me3Al + 3H2O → Al2O3 + 3CH4
The highest growth rate obtained with this route is about 1.2 Å/cycle, with a deposition temperature between 150°C and 450°C. With H2O2 the growth rate is in the same order, but using other sources it is lower.
Aluminium chloride (AlCl3) has also been used as aluminum source, coupled with H2O, O2 or alcohols as oxygen sources. The growth rate in this case is typically in the range 0.4 – 0.9 Å/cycle, but it is variable not only according to the co-reactant chosen for AlCl3, but also to the reactor and the deposition temperature.
Water has been tested also with dymethylaluminum choride (Me2AlCl), giving a maximum growth rate of 0.8 Å/cycle at 250°C .